292 T. Maiyalagan, B. Viswanathan / Materials Chemistry and Physics 93 (2005) 291–295
used a combination of CVD and template synthesis methods
to synthesize highly aligned, uniform, hollow and open
ended (suitable for ﬁlling with other materials) CNTs with
diameters ranging from 20 to 200 nm. Among all the methods
of preparation of CNTs, the template synthesis method has
the advantage of controlling composition, morphology and
the size of the nanotubes . Nitrogen containing carbon
nanotubes prepared by template synthesis using precursors
such as polyacrylonitrile  and polypyrrole , have
In this letter, use of polyvinylpyrrolidone as a new precur-
sor for the synthesis of nitrogen containing carbon nanotubes
by template synthesis is discussed. The well-aligned nitrogen
containing CNTs have been formed. The morphology and
structural features of the nanotubes have been investigated
using electron microscopy and Raman spectroscopy. The
composition and bonding of the nanotubes were determined
using IR and X-ray photoelectron spectroscopy (XPS).
All the chemicals used were of analytical grade.
Polyvinyl pyrrolidone (Sisco Research Laboratories, India),
dichloromethane and concentrated HF (both from Merck)
were used. Alumina template membranes were obtained from
Whatman Anopore Filters.
2.2. Synthesis of nitrogen containing carbon nanotubes
Polyvinylpyrrolidone (PVP, 5 g) was dissolved in
dichloromethane (20 ml) and impregnated directly into the
pores of the alumina template by wetting method . After
complete solvent evaporation, the membrane was placed in a
quartz tube (30 cm length, 3.0 cm diameter) kept in a tubular
furnace and carbonized at 1173 K under Ar gas ﬂow. After
3 h of carbonization, the quartz tube was naturally cooled to
room temperature. The resulting carbon–nitrogen compos-
ite was immersed in 48% HF at room temperature for 24 h
to remove the alumina template and the nitrogen containing
CNTs were obtained as an insoluble fraction. The nanotube
were then washed with distilled water to remove the residual
HF and was dried at 393 K.
The total chemical composition of the nanotubes was de-
termined by elemental analysis using Hereaus CHN analyzer
after the removal of alumina template. The scanning electron
micrographs were obtained using JEOL JSM-840 model
working at 15 keV. For transmission electron microscopic
studies, the nanotubes dispersed in ethanol were drop cast
on to a carbon-coated copper grid followed by solvent
evaporation in air at room temperature and the images were
obtained using Phillips 420 model, operating at 120 keV. The
nanotubes were sonicated in acetone for 20 min and then
were dropped on cleaned Si substrates and AFM imaging
was performed in air using a Nanoscope IIIA atomic force
microscope (Digital Instruments, St. Barbara, CA) operated
in contact mode.
The CNTs placed in glass capillary tubes were used
for recording Raman spectrum at the room temperature
with 514.5 nm excitation in backscattered mode using
Bruker FRA106 FT-Raman instrument. The IR spectrum
was recorded with Perkin-Elmer (L-710) spectrophotome-
ter. The X-ray photoelectron spectroscopic analysis was car-
ried out using VG ESCALAB 220 iXL instrument at Al K␣
(1486.5 eV) radiation.
3. Results and discussion
Elemental analysis was ﬁrst conducted to examine
whether nitrogen has really entered the carbon nanotube
framework. It has been found that the samples prepared con-
tained about 87.2% carbon and 6.6% nitrogen (w/w).
Scanning electron microscopic images given in Fig. 1
shows the morphology of the nitrogen containing CNTs after
the removal of alumina template. The nanotubes are aligned
and grouped into high-density arrays, appearing like the bris-
tles of a brush (Fig. 1a) and this reﬂects the highly dense
straight pores of the alumina membrane (∼109 pores cm−2).
Images b and c of Fig. 1 show the lateral view of the well-
aligned nanotubes of the length 50–60 m with open ends
(indicated by arrows in Fig. 1c) similar to the thickness of
the alumina membranes. Moreover, we performed transmis-
sion electron microscopy (TEM) analysis to determine the
morphology and the diameter of the nanotube.
Transmission electron microscopy images of the
nitrogen containing carbon nanotubes prepared from
polyvinylpyrrolidone are shown in Fig. 2. The carbonized
specimens are found to have a hollow structure with open
ends. Because the channels of the membranes being cylin-
drical with uniform diameter and the tube diameter closely
matching the pore size of the template used, monodispersed
nanotubes of the desired material were obtained. Since no
catalyst has been used for synthesis of nitrogen containing
carbon nanotubes, it is worth pointing out that the nanotubes
produced by template synthesis under normal experimental
conditions are almost free from impurities.
AFM images of the nitrogen containing carbon nanotubes
deposited on a silicon substrate are shown in Fig. 3. The AFM
tip was carefully scanned across the tube surface in a direction
perpendicular to the tube axis. From the AFM images, a part
of the long nanotube is appeared to be cylindrical in shape
and to be terminated by a symmetric hemispherical cap.
Raman spectrum is a unique tool to characterize the
nanotubes under study, since the amount of ordering and
degree of sp2 and sp3 bonding leaves a characteristic Raman
“ﬁnger print”. Thus, the graphitic nature of the nitrogen
T. Maiyalagan, B. Viswanathan / Materials Chemistry and Physics 93 (2005) 291–295 293
Fig. 1. SEM images of the nitrogen containing carbon nanotubes: (a) the top view of the nanotubes, (b) side view of the vertically aligned nanotubes and (c)
high-magniﬁcation lateral view of the nanotubes.
containing carbon nanotubes obtained from the carboniza-
tion of polyvinylpyrrolidone was investigated by Raman
spectroscopy. Fig. 4 shows Raman spectrum of the sample.
It shows two peaks at 1290 and 1590 cm−1. The peak at
1590 cm−1 (G-band) corresponds to the high frequency E2g
ﬁrst-order mode, which can be attributed to the opposing
movement of two-neighboring carbon atoms in a graphite
sheet [29,30]. The peak at 1290 cm−1 (D-band) could be as a
result of defects in the curved graphitic sheets, tube ends and
ﬁnite size crystalline domains of the tubes . The D-band
appears to be signiﬁcantly stronger than the G-band indicat-
ing the amorphization of the graphite network is due to much
higher nitrogen content in the carbon nanotubes .
Although the carbon nanotubes prepared from
polyvinylpyrrolidone show graphitic band, they have lesser
graphitic structure as judged from the intensity and line width
of the peak. And the carbonized specimen is found to have
a poorly ordered graphite structure in the form of a hollow
The nature of chemical bonding between the elements
was analyzed using infrared and X-ray photoelectron
spectroscopic techniques. Infrared spectrum of the nitrogen
containing carbon nanotubes is similar to those reported for
other carbon nitride materials . FT-IR spectrum (Fig. 5)
Fig. 2. (a) TEM image of the nitrogen containing carbon nanotubes and (b) higher magniﬁcation image of the individual nanotube (an arrow indicating the
open end of the tube).
294 T. Maiyalagan, B. Viswanathan / Materials Chemistry and Physics 93 (2005) 291–295
Fig. 3. AFM image of the nitrogen containing carbon nanotubes.
shows the stretching and deformation mode of NH2 group
at 3420 and 1640 cm−1, respectively. The peaks at 2928
and 2855 cm−1 were observed only in amorphous CNTs
and were assigned to C–H bonding [33,34]. Moreover,
the presence of nitrogen in the carbon nanotubes induces
CNTs to show G- and D-bands in FT-IR spectrum. The
Peak at 1594 cm−1 is attributed to C N stretching modes
[35,36], while the other sharp peaks at 1381, 1124 and
1084 cm−1 corresponds to the characteristic absorbance of
single C–N bonds . These are the strong evidences of
incorporated nitrogen in the carbon nanotubes. And also a
band at 780 cm−1 is attributed to graphitic sp2 domains .
The composition and the nature of chemical bonding of
the prepared nanotube sample were studied by XPS mea-
surement. The gross chemical composition estimated from
the XPS results gave an N/C ratio of about 0.06. The decon-
voluted C 1s and N 1s XPS spectra of nitrogen containing
Fig. 4. Raman spectrum of the nitrogen containing carbon nanotubes.
carbon nanotubes are shown in Fig. 6. The C 1s can be de-
convoluted in to two lines peaked at 284.5 and 287.05 eV. By
comparing with urotropine (C6H12N4, sp3 binding energy:
286.9 eV)  and pyridine (C5H5N, sp2 binding energy:
285.5 eV) , the carbon peak at 287.05 and 284.5 eV are
assigned due to sp3 and sp2 bondings, respectively. The N
1s also can be deconvoluted in to two lines peaked at 397.6
and 399.4 eV. These two peaks are attributed to sp2 N, i.e.
substitutional N in the graphite sheet . The observed C
1s and N 1s binding energies are comparable to those found
in melamine (C3N6H6) molecules with covalent C–N bonds,
which is similar to the C–N bonds of graphitic carbon nitride
(C3N4) . Together with the XPS results, it is inferred that
the nitrogen atom is chemically bonded to the three neigh-
boring carbons in a graphitic basal plane, and therefore the
presence of the nitrogen in the carbon framework is con-
Fig. 5. FT-IR spectrum of the nitrogen containing carbon nanotubes.
T. Maiyalagan, B. Viswanathan / Materials Chemistry and Physics 93 (2005) 291–295 295
Fig. 6. XPS spectra of the nitrogen containing carbon nanotubes after the removal of alumina template: (a) C 1s and (b) N 1s.
In summary, polyvinylpyrrolidone is a highly efﬁcient
polymer precursor for synthesis of nitrogen containing car-
bon nanotubes and the adopted template method is effective
for the synthesis of well-aligned nitrogen containing carbon
nanotubes with control over the packing density. The nitrogen
containing carbon nanotubes with controlled morphology
and composition has been achieved. The morphology of the
aligned nanostructures has been veriﬁed by SEM, TEM and
AFM. Raman spectroscopic studies show a higher degree
of disorder, indicates a distortion of the graphitic network
is due to nitrogen incorporation in the carbon nanotubes.
The presence of carbon–nitrogen bond in CNTs has been
conﬁrmed by infrared spectrum and XPS analysis.
 S. Ijima, Nature 354 (1991) 56.
 M.M.J. Treacy, T.W. Ebbesen, J.M. Gibson, Nature 381 (1996) 678.
 S.T. Trans, A.R.M. Verscheren, C. Dekker, Nature 393 (1998) 49.
 S.S. Wong, E. Joselevich, A.T. Woolley, C.L. Cheung, C.M. Lieber,
Nature 394 (1998) 52.
 S.S. Fan, M.G. Chapline, N.R. Franklin, T.W. Tombler, A.M. Cassell,
H.J. Dai, Science 283 (1999) 512.
 J.M. Planeix, N. Coustel, B. Coq, V. Brotons, P.S. Kumbhar, R.
Dutartre, P. Geneste, P. Bernier, P.M. Ajayan, J. Am. Chem. Soc.
116 (1994) 7935.
 C. Niu, E.K. Sichel, R. Hoch, D. Moy, H. Tennent, Appl. Phys. Lett.
70 (1997) 1480.
 C.Y. Liu, A.J. Bard, F. Wudl, I. Weitz, J.R. Heath, Electrochem.
Solid State Lett. 2 (1999) 577.
 C. Wang, M. Waje, X. Wang, J.M. Tang, R.C. Haddon, Y.S. Yan,
Nano Lett. 4 (2004) 345.
 O. Stephan, P.M. Ajayan, C. Colliex, Ph. Redlich, J.M. Lambert, P.
Bernier, P. Leﬁn, Science 266 (1994) 1683.
 M. Glerup, M. Castignolles, M. Holzinger, G. Hug, A. Loiseau, P.
Bernier, Chem. Commun. (2003) 2542.
 M. Terrones, P.M. Ajayan, F. Banhart,.X. Blase, D.L. Carroll, J.C.
Charlier, R. Czerw, B. Foley, N. Grobert, R. Kamalakaran, P. Kohler-
Redlich, M. Ruhle, T. Seeger, H. Terrones, Appl. Phys. A Mater. 74
 R. Czerw, M. Terrones, J.-C. Charlier, X. Blase, B. Foley, R. Ka-
malakaran, N. Grobert, H. Terrones, D. Tekleab, P.M. Ajayan, W.
Blau, M. Ruehle, D.L. Carroll, Nano Lett. 9 (2001) 457.
 A.K. Shukla, M.K. Ravikumar, A. Roy, S.R. Barman, D.D. Sarma,
A.S. Arico, V. Antonucci, L. Pino, N. Giordano, J. Electrochem.
Soc. 141 (1994) 517.
 S.C. Roy, P.A. Christensen, A. Hamnett, K.M. Thomas, V. Trapp, J.
Electrochem. Soc. 143 (1996) 3073.
 M. Glerup, J. Steinmetz, D. Samaille, O. Stephan, S. Enouz,
A. Loiseau, S. Roth, P. Bernier, Chem. Phys. Lett. 387 (2004)
 Y. Zhang, H. Gu, K. Suenaga, S. Iijima, Chem. Phys. Lett. 279
 D. Golberg, Y. Bando, W. Han, K. Kurashima, T. Sato, Chem. Phys.
Lett. 308 (1999) 337.
 C. Tang, Y. Bando, D. Golberg, F. Xu, Carbon 42 (2004) 2625.
 K. Suenaga, M. Yudasaka, C. Colliex, S. Iijima, Chem. Phys. Lett.
316 (2000) 365.
 C.R. Martin, Science 266 (1994) 1961.
 B. Rajesh, K. Ravindranathan, J.-M. Thampi, N. Bonard, H.J. Xan-
thopoulos, B. Mathieu, Viswanathan, J. Phys. Chem. B 107 (2003)
 G. Che, B.B. Lakshmi, C.R. Martin, E.R. Fisher, R.A. Ruoff, Chem.
Mater. 10 (1998) 260.
 T. Kyotani, L.-F. Tsai, A. Tomita, Chem. Mater. 7 (1996)
 R. Che, L.-M. Peng, Q. Chen, X.F. Duan, Z.N. Gu, Appl. Phys. Lett.
82 (2003) 331.
 R.V. Parthasarathy, K.L.N. Phani, C.R. Martin, Adv. Mater. 7 (1995)
 J. Jang, J.H. Oh, Chem. Commun. (2004) 882.
 M. Steinhart, J.H. Wendorff, A. Greiner, R.B. Wehrspohn, K.
Nielsch, J. Schilling, J. Choi, U. Goesele, Science 296 (2002) 1997.
 F. Tuinstra, J.L. Koenig, J. Chem. Phys. 53 (1970) 1126.
 R.J. Nemanich, S.A. Solin, Phys. Rev. B 20 (1979) 392.
 S. Choi, K.H. Park, S. Lee, K.H. Koh, J. Appl. Phys. 92 (2002)
 V.N. Khabashesku, J.L. Zimmerman, J.L. Margrave, Chem. Mater.
12 (2000) 3264.
 Y.J. Bai, B. Lu, Z.G. Liu, Z. G. J. Cryst. Growth 247 (2003) 505.
 M. Barber, J.A. Connor, M.F. Guest, I.H. Hillier, M. Schwarz, M.
Stacey, J. Chem. Soc. Faraday Trans. II 69 (1973) 551.
 Y. Qiu, L. Gao, Chem. Commun. (2003) 2378.
 J.H. Kaufman, S. Metin, D.D. Saperstein, Phys. Rev. B 39 (1989)
 X.A. Zhao, C.W. Ong, Y.C. Tsang, Y.W. Wong, P.W. Chan, C.L.
Choy, Appl. Phys. Lett. 66 (66) (1995) 2652.
 U. Gelius, R.F. Heden, J. Hedman, B.J. Lindberg, R. Manne, R.
Nordberg, R. Nordling, K. Siegbahn, Phys. Scr. 2 (1970) 70.
 A. Johansson, S. Stafstrom, J. Chem. Phys. 111 (1999) 3203.
 A.P. Dementjev, A. De Graaf, M.C.M. Van de Sanden, K.I.
Maslakov, A.V. Naumkin, A.A. Serov, Diam. Relat. Mater. 9 (2000)